#------------------------------------------------------------------------------
#$Date: 2025-07-06 14:53:35 +0200 (Sun 06 de Jul de 2025) $
#$Revision: 300415 $
#$URL: svn://www.crystallography.net/cod/cif/7/13/44/7134436.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7134436
loop_
_publ_author_name
'Drushliak, Viktoriia'
'Szafrański, Marek'
_publ_section_title
;
 Effect of pressure and temperature on the structure and optical
 properties of two-dimensional lead iodide perovskites
;
_journal_issue                   44
_journal_name_full               'Chemical Communications'
_journal_page_first              8019
_journal_page_last               8022
_journal_paper_doi               10.1039/D5CC01232E
_journal_volume                  61
_journal_year                    2025
_chemical_formula_sum            'C H6 Cs I4 N3 Pb'
_chemical_formula_weight         907.79
_chemical_name_systematic        'Cesium guanidinium lead tetraiodide'
_space_group_crystal_system      orthorhombic
_space_group_IT_number           58
_space_group_name_Hall           '-P 2 2n'
_space_group_name_H-M_alt        'P n n m'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     heavy
_audit_creation_date             2024-10-23
_audit_creation_method
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_audit_update_record
;
2025-03-03 deposited with the CCDC.	2025-04-23 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   18.043(8)
_cell_length_b                   12.2374(4)
_cell_length_c                   11.7887(4)
_cell_measurement_pressure       1920000(30000)
_cell_measurement_reflns_used    3581
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.1200
_cell_measurement_theta_min      1.7300
_cell_volume                     2602.9(12)
_computing_cell_refinement       'CrysAlisPro 1.171.41.93a (Rigaku OD, 2020)'
_computing_data_collection       'CrysAlisPro 1.171.41.93a (Rigaku OD, 2020)'
_computing_data_reduction        'CrysAlisPro 1.171.41.93a (Rigaku OD, 2020)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXS  (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.3200
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.357
_diffrn_measured_fraction_theta_max 0.278
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  φ    -35.00  19.75   0.75   70.00   0.00 -30.00   0.00    --    73
  2  φ    140.00 200.00   0.75   70.00   0.00 -30.00   0.00    --    80
  3  φ    160.00 217.00   0.75   70.00   0.00  30.00   0.00    --    76
  4  φ    -20.00  34.75   0.75   70.00   0.00  30.00   0.00    --    73
  5  ω    -24.00  24.00   0.75   70.00    --   30.00  39.46 -12.90   64
  6  ω    -24.00  24.00   0.75   70.00    --   30.00  39.46 167.10   64
  7  ω    -50.00  10.00   0.75   70.00    --  -30.00  39.46 167.10   80
  8  ω    -50.00  10.00   0.75   70.00    --  -30.00  39.46 -12.90   80
  9  ω    -64.00  -8.50   0.75   70.00    --  -30.00  81.40 -28.90   74
 10  ω    -64.00  -8.50   0.75   70.00    --  -30.00  81.40 151.10   74
 11  ω    -19.00   8.00   0.75   70.00    --   30.00  81.40 151.10   36
 12  ω    -19.00   8.00   0.75   70.00    --   30.00  81.40 -28.90   36
 13  ω    -43.00 -21.25   0.75   70.00    --   30.00 134.60 -56.90   29
 14  ω    -43.00 -21.25   0.75   70.00    --   30.00 134.60 123.10   29
 15  ω    -90.00 -36.00   0.75   70.00    --  -30.00 134.60 123.10   72
 16  ω    -90.00 -36.00   0.75   70.00    --  -30.00 134.60 -56.90   72
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini ultra'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0382172971
_diffrn_orient_matrix_UB_12      -0.0098896138
_diffrn_orient_matrix_UB_13      -0.0085729651
_diffrn_orient_matrix_UB_21      -0.0082031837
_diffrn_orient_matrix_UB_22      -0.0280614035
_diffrn_orient_matrix_UB_23      -0.0512273769
_diffrn_orient_matrix_UB_31      0.0030122268
_diffrn_orient_matrix_UB_32      0.0498149430
_diffrn_orient_matrix_UB_33      -0.0305721696
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0388
_diffrn_reflns_av_unetI/netI     0.0220
_diffrn_reflns_Laue_measured_fraction_full 0.357
_diffrn_reflns_Laue_measured_fraction_max 0.278
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            10780
_diffrn_reflns_point_group_measured_fraction_full 0.357
_diffrn_reflns_point_group_measured_fraction_max 0.278
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.825
_diffrn_reflns_theta_min         2.399
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    25.164
_exptl_absorpt_correction_T_max  0.248
_exptl_absorpt_correction_T_min  0.115
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.93a (Rigaku Oxford Diffraction, 2020)
Numerical absorption correction based on gaussian integration over
a multifaceted crystal model (Absorb Angel (2004) J. Appl. Cryst. 37:486-492)
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    4.633
_exptl_crystal_description       plate
_exptl_crystal_F_000             3056
_exptl_crystal_preparation       'mounted in a diamond-anvil cell '
_exptl_crystal_size_max          0.182
_exptl_crystal_size_mid          0.140
_exptl_crystal_size_min          0.044
_refine_diff_density_max         0.779
_refine_diff_density_min         -0.703
_refine_diff_density_rms         0.163
_refine_ls_extinction_coef       0.000074(16)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.259
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     82
_refine_ls_number_reflns         991
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.259
_refine_ls_R_factor_all          0.0585
_refine_ls_R_factor_gt           0.0317
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0172P)²+24.7927P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0627
_refine_ls_wR_factor_ref         0.0726
_reflns_Friedel_coverage         0.000
_reflns_number_gt                620
_reflns_number_total             991
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d5cc01232e2.cif
_cod_data_source_block           CsGPbI4_1_92
_cod_depositor_comments
'Adding full bibliography for 7134427--7134444.cif.'
_cod_original_cell_volume        2602.9(11)
_cod_database_code               7134436
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.433
_shelx_estimated_absorpt_t_min   0.093
_exptl_absorpt_special_details
; 
Data were collected at room temperature and pressure of 1.92(3) GPa
(1920000 kPa). 
Pressure was determined by monitoring the shift of the ruby
R1-fluorescence line.
"_diffrn_measured_fraction_theta_full" value is low, because 
the access to the reciprocal space is restricted due to the use of
the diamond anvil cell.
;
_exptl_oxdiff_absorpt_process_details
;
Gaussian integration over a grid
of 16 x 16 x 16 points =  4096 total grid points
  Based upon method of Burnham (1966)

 Data corrected for diamond-anvil cell absorption
 Note that exptl_absorpt_correction_tmin and _tmax
 the total correction factors applied to the intensities
 The individual factors are: 
         range of dac transmission factors (min-max)      0.694     0.726
         range of gasket transmission (min-max)           0.558     1.000
         range of P media transmission (min-max)          1.000     1.000

 thickness of diamond anvil 1:  8.000 mm, mu =  0.0200 mm-1
       thickness of platten 1:  0.000 mm, mu =  0.0000 mm-1

 thickness of diamond anvil 2:  8.000 mm, mu =  0.0200 mm-1
       thickness of platten 2:  0.000 mm, mu =  0.0000 mm-1

    Gasket shadowing corrections were made based upon
    Gasket thickness = 300.0 microns, radius = 163.0 microns
    Gasket absorption coeff =        30.30 mm-1
    REFLECTION WAS CONSIDERED TOTALLY OBSCURED IF 
 FRACTION CRYSTAL ILLUMINATED WAS LESS THAN 0.00

    Non-absorbing pressure medium
;
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All N(H) groups, All N(H,H) groups
2. Others
 Fixed Sof: H12A(0.5) H12B(0.5)
 Fixed X: H22(0.55893)
 Fixed Y: H22(0.12215)
 Fixed Z: H22(0.062429)
3.a X=CH2 refined with riding coordinates:
 N11(H11A,H11B), N12(H12A,H12B), N21(H21A,H21B)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.386
_oxdiff_exptl_absorpt_empirical_full_min 0.687
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x-1/2, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pb1 Pb 0.25098(8) 0.87509(7) 0.25135(4) 0.0272(11) Uani 1 1 d . . . . .
Cs1 Cs 0.4098(2) 0.62416(14) 0.500000 0.037(2) Uani 1 2 d S T P . .
I1 I 0.42055(16) 0.87792(9) 0.31069(8) 0.0370(19) Uani 1 1 d . . . . .
I2 I 0.07920(15) 0.87282(9) 0.19543(8) 0.0369(18) Uani 1 1 d . . . . .
Cs2 Cs 0.3917(2) 1.12529(13) 0.500000 0.040(2) Uani 1 2 d S T P . .
I3 I 0.24876(16) 1.12460(8) 0.20094(10) 0.0451(17) Uani 1 1 d . . . . .
I4B I 0.2190(3) 0.93562(14) 0.500000 0.048(3) Uani 1 2 d S T P . .
I5A I 0.2777(3) 0.81574(14) 0.000000 0.042(3) Uani 1 2 d S T P . .
C1 C -0.042(4) 0.884(2) 0.500000 0.029(8) Uiso 1 2 d S . P . .
N11 N -0.0765(16) 0.8832(9) 0.4025(10) 0.035(4) Uiso 1 1 d . . . . .
H11A H -0.051879 0.875900 0.340436 0.042 Uiso 1 1 calc R U . . .
H11B H -0.123900 0.890120 0.400414 0.042 Uiso 1 1 calc R U . . .
N12 N 0.032(3) 0.8727(16) 0.500000 0.034(7) Uiso 1 2 d S . P . .
H12A H 0.055607 0.865524 0.436936 0.040 Uiso 0.5 1 calc R U P . .
H12B H 0.056105 0.872804 0.563064 0.040 Uiso 0.5 1 calc R U P . .
C2 C 0.460(4) 0.116(2) 0.000000 0.034(9) Uiso 1 2 d S . P . .
N21 N 0.4281(19) 0.1135(11) 0.0964(12) 0.055(5) Uiso 1 1 d . . . . .
H21A H 0.380644 0.109390 0.100618 0.066 Uiso 1 1 calc R U . . .
H21B H 0.454261 0.115764 0.157422 0.066 Uiso 1 1 calc R U . . .
N22 N 0.535(4) 0.1239(18) 0.000000 0.037(7) Uiso 1 2 d S . P . .
H22 H 0.558930 0.122150 0.062429 0.044 Uiso 1 1 d . U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
3 -1 16 0.0746
-3 1 -16 0.0636
-5 -17 -2 0.0679
5 17 4 0.1066
1 14 -10 0.0858
5 10 13 0.0855
-25 3 2 0.0220
25 -3 -2 0.0220
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
I1 Pb1 I2 179.12(3) . . ?
I3 Pb1 I1 88.23(6) 3_545 . ?
I3 Pb1 I1 92.54(6) . . ?
I3 Pb1 I2 91.74(6) 3_545 . ?
I3 Pb1 I2 87.49(6) . . ?
I3 Pb1 I3 179.10(4) 3_545 . ?
I4B Pb1 I1 88.15(9) . . ?
I4B Pb1 I2 90.98(9) . . ?
I4B Pb1 I3 86.75(4) . . ?
I4B Pb1 I3 93.73(4) . 3_545 ?
I4B Pb1 I5A 178.15(14) . . ?
I5A Pb1 I1 93.68(9) . . ?
I5A Pb1 I2 87.20(9) . . ?
I5A Pb1 I3 92.84(4) . . ?
I5A Pb1 I3 86.65(4) . 3_545 ?
Pb1 I3 Pb1 158.57(4) 3 . ?
Pb1 I4B Pb1 144.49(12) 6_556 . ?
Pb1 I5A Pb1 147.21(11) . 6 ?
N11 C1 N11 123(6) . 6_556 ?
N12 C1 N11 118(3) . 6_556 ?
N12 C1 N11 118(3) . . ?
C1 N11 H11A 120.0 . . ?
C1 N11 H11B 120.0 . . ?
H11A N11 H11B 120.0 . . ?
C1 N12 H12A 120.0 . . ?
C1 N12 H12B 120.0 . . ?
H12A N12 H12B 120.0 . . ?
N21 C2 N21 127(7) . 6 ?
N21 C2 N22 117(4) . . ?
N21 C2 N22 117(4) 6 . ?
C2 N21 H21A 120.0 . . ?
C2 N21 H21B 120.0 . . ?
H21A N21 H21B 120.0 . . ?
C2 N22 H22 121(4) . . ?
C2 N22 H22 121(4) . 6 ?
H22 N22 H22 118(7) . 6 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pb1 I1 3.139(3) . ?
Pb1 I2 3.169(3) . ?
Pb1 I3 3.1165(12) 3_545 ?
Pb1 I3 3.1110(12) . ?
Pb1 I4B 3.0778(11) . ?
Pb1 I5A 3.0887(10) . ?
C1 N11 1.31(4) . ?
C1 N11 1.31(4) 6_556 ?
C1 N12 1.34(8) . ?
N11 H11A 0.8600 . ?
N11 H11B 0.8600 . ?
N12 H12A 0.8600 . ?
N12 H12B 0.8600 . ?
C2 N21 1.27(4) . ?
C2 N21 1.27(4) 6 ?
C2 N22 1.35(9) . ?
N21 H21A 0.8600 . ?
N21 H21B 0.8600 . ?
N22 H22 0.86(3) . ?
N22 H22 0.86(3) 6 ?
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
3.2641 -0.9962 16.4273 -0.0062 -0.8403 -0.5420
-3.1741 1.3417 -16.4119 0.0061 0.8291 0.5590
-4.5900 -16.8606 -1.6746 0.0057 0.5966 -0.8025
4.9008 16.5046 3.5452 -0.0063 -0.6850 0.7286
1.2666 13.6493 -10.0932 -0.0001 0.1236 0.9923
5.2640 9.5955 13.3491 -0.0082 -0.9963 0.0857
-24.8712 2.9548 2.3641 -1.0000 0.0000 0.0000
24.8712 -2.9548 -2.3641 1.0000 0.0000 0.0000
